1.3 Low cost optical components
1.3.2 Short wavelength VCSEL technology
The first concept about the possibility of realizing lasers devices which could emit in the direction perpendicular to the wafer surface was proposed in 1977 by Prof. Kenichi Iga .
The necessity of having such new type of lasers came up to solve some issues related to Edge Emitting Lasers (EELs). For example, the impossibility of testing the latter devices before cutting the wafer and separating into chips, or the limitation on the monolithically integration of such lasers into optical circuits due to the finite cavity length .
Figure 1.14: Top view of a VCSEL.
Since this first publication, VCSELs have been studied by many researchers which gave important contribution to the improvement of this technology. In particular, in 1989 J.Jewell reported the first full-monolithic VCSEL composed of epitaxially grown Distributed Bragg Reflectors (DBR) and InGaAs-GaAs Quantum Wells (QWs) active region . As it will be explained in a later section, the realization of regular Multi-Quantum Wells (MQWs) lead to the important reduction of threshold current keeping high the output optical power.
Therefore, thank to their overall benefits, MQWs became a constant presence in VCSEL active regions. Note that this type of technology is not exclusive of VCSELs but it is used also in EEL [46, 47]. The success of MQWs-based VCSELs came at the same time with the development of manufacturing techniques such as Metal-Organic Chemical Vapor Depo-sition (MOCVD) and Molecular Beam Epitaxy (MBE) which give the possibility of growing materials with very small thickness and high precision.
In fact, these two techniques allow to control the material grown layer by layer, realiz-ing structures with a precise doprealiz-ing and sharp interfaces between different materials. With thickness of few nanometers, electron’s De Broglie wavelength is comparable with the spatial dimensions, at least in one of the three directions, and quantum effects are observed. Quan-tum wires and quanQuan-tum dots are present if, respectively, two or three dimensions are involved.
Instead, QWs occurs in heterostructures realized with materials of different energy bandgap, e.g. GaAs and GaAlAs.
Realizing more than one QW increases the gain, and implies less consumption of bias current than a bulk laser beacuse of the smaller volume of the active region. The PIN-type doping scheme is similar to conventional EELs. In the most simple device layouts, electric current is
injected from ohmic contacts on the top epitaxial side and the backside of the substrate .
Nowadays VCSELs are a well–consolidated technology which is already present in many ap-plications such as the high-speed communications in data-centers [49–51] or proximity sensors in mobile devices  as for example the iPhone provided by Apple  .
VCSELs vs. EELs
𝐼𝐼𝑁𝐽 Ohmic contacts
Confinement region p-type
Figure 1.15: Typical structure of GaAs VCSEL (a) and EEL (b).
As the name says, the main characteristic of a VCSEL is the emission direction of the light, which is not from the edge, like other kinds of laser such as Distributed Feed-Back (DFB) or Fabry-Perot (FP), but it is from the top of the structure (see Figure 1.15). This fact gives many advantages compared to EELs: first of all the production cost can be reduced thanks to the possibility of realizing several tens of thousand of VCSELs in the same wafer and testing directly on it. This, indeed, is not possible for EEL for which the wafer must be sliced to test the behavior of each sample from the edge, increasing the time and cost of the testing reliability process. Moreover, because of the compact size of VCSEL, typically 250×250µm2 there could be more devices on a wafer than EEL and therefore the production could be done in larger quantities without any type of additional cost.
Summarizing, the advantages of VCSELs compared to EEL are:
• Lower threshold current;
• Higher efficiency but lower emitted power;
• Lower cost;
• Possibility of creating VCSEL arrays without any additional manufacturing cost;
• Higher density of chips in one wafer;
• Narrow beam divergence and circularly symmetric profile;
• Higher modulation bandwidth due to the short photons lifetime, which leads to a high oscillation relaxation frequency.
• Easier matching at typical RF impedance (50 Ω or 75 Ω) VCSEL physical structure and behavior
𝑛𝑒𝑓𝑓,2 𝑛𝑒𝑓𝑓,1 Δ𝑛𝑒𝑓𝑓
Oxidation layer Active layer
Bottom DBR Top DBR
Inner cavity 𝐿
p-DBR Barrier n-DBR
Barrier region QW
Figure 1.16: Side view of a VCSEL (a) and example of single QW active region (b).
Next, the physics of VCSELs is described in some details for a better understanding of their properties and behavior.
The physical structure of GaAs VCSELs is composed by the following components:
Top and bottom DBR: DBRs are typically used to generate a resonant cavity. They consist of alternating pairs of semiconductor materials (generally alloys) having different re-fractive index. In the case of VCSEL operating at 850 nm or 980 nm the material employed is typically AlxGaAs1 –x in which the parameter x changes between the two layers. This differ-ence causes a refractive index separation between the layers. The layer thickness is designed to be λ/4n where n is the layer refractive index and λ is the desired resonant wavelength.
Because of the current flow from the contact through the mirrors, they are also doped to reduce the series resistance . Moreover a single-step grading with 5 nm thick layers of intermediate bandgap energy is used to reduce the electrical series resistance  realizing a graded-DBR. Finally, the bottom DBR has more reflectivity than the top one, to let the light go out only in one direction.
Active region: for the laser operating in the wavelength considered ('850 nm), the ac-tive structure is composed generally of few QWs realized in GaAs with some 10nm thickness.
In particular the active region consists of half-wavelength thick Al0.2Ga0.8As with three 8 nm thick unstrained GaAsQWs separated by 10 nm barriers in the center. Quarter-wavelength Al0.5Ga0.5As cladding layers are introduced on both sides of the active region to improve longitudinal carrier confinement .
Confinement region: it is responsible for the confinement of the electrons in the active region. Actual VCSELs adopts oxide or double-oxide confinement with unrivaled perfor-mance [56, 57], exploiting selective lateral oxidation of an about 30 nm thick AlAs. This technology has replaced the initial most common technique based on proton implantation, because of the higher optical losses in the cavity of the latter compared to the oxide [56, 58].
VCSEL emission spectrum behavior
In this paragraph, the emission optical spectrum of VCSELs is analyzed in detail. Their small effective cavity length in the emission direction guarantees only one longitudinal mode within the cavity. Indeed, when the wavelengthλis fixed ('850 nm), only a set of lengthsL is admitted to have the resonance condition. In particular, the following condition is necessary for the inner cavity length:
2¯nm m= 1,2,3... (1.7)
in which ¯n is the spatial average refractive index. For VCSELs typically is m= 2, since for L = 2¯λn the current injection efficiency results to be low . This results in L = λn¯ which for the case of λ = 850 nm and ¯n ' 3.6 (e.g. GaAs) leads to L ' 236.11 nm. This value regards theinner cavity length (distance between top and bottom DBR). However, the actual cavity that is present in VCSELs takes into account also the presence of the two mirrors. In particular, an effective lengthlef f for both mirrors can be calculated, making the assumption that the reflection effectively originates from a hard mirror with identical peak reflectivity placed at a distance lef f. From this consideration it is possible to define a effective cavity lengthLef f defined as:
Lef f =L+lef f,t+lef f,b (1.8)
wherelef f,t andlef f,b are top and bottom DBR effective length, respectively. Therefore Lef f depends on the DBR properties (e.g. number of mirror pairs) and generally is in the order of 1µm [48, 59].
The longitudinal mode spacing among the possible wavelength for a cavity of lengthLef f is given by :
2¯nLef f (1.9)
Therefore, sinceLef f is of the same order of magnitude ofλin VCSELs, a large spacing among the possible propagation wavelengths occurs, resulting in ∆λ'110 nm. This value is much larger than the material gain bandwidth, which is in general about 50 nm, and consequently only a single longitudinal mode emission is allowed.
However, due to the transverse size of the device an actual multimode emission occurs. A cylindrical structure is typically created withDa= 2aas aperture diameter (see Figure 1.16).
The oxidized layer, which is used for confining the injected current, also lowers the refractive index (from ∼ 3 to ∼ 1.6 at wavelength of 850nm ). This provides transverse optical
confinement, forming a waveguide for light which propagates in the longitudinal direction.
Applting the effective index analysis given by Hadley  it is possible to understand the presence of a waveguide. This analysis assumes that any modification of the VCSEL resonator that produces a local shift of the resonance wavelength ∆λ0 produces a corresponding change of the effective index ∆nef f (see Figure 1.16) in that region for which holds the relation:
nef f ≈ ∆λ0
Because the oxidation layer lowers the effective refractive index of the material, it is
∆λ0 < 0 and therefore nef f,2 < nef f,1. Therefore, a cylindrical waveguide of diameter Da
having an effective refractive index difference ∆nef f is present, which allows to apply the theory of the step-index optical fiber for analyzing the guiding characteristics. Therefore, assuming the weakly guiding approximation ∆nef f << nef f the modes can be expressed in terms of linearly polarized modes LPl,p in whichl and p are the azimuthal and radial mode numbers, respectively. Because of the blue-shift given by the oxidation layer the fundamental mode LP01is the one with higher wavelength compared to the higher order ones. An example of emission spectrum for different biasing conditions of a VCSEL is shown in Figure 1.17.
850 851 852 853 854 855
850 851 852 853 854 855
850 851 852 853 854 855
Figure 1.17: Example of optical spectrum measured for a typical oxide confined MTM VCSEL realized on GaAs. The spectrum is measured forIbias'Ith, Ibias'(Is−Ith)/2 and Ibias'Is current for the real wavelength.
Indeed, it should be pointed out that any deviation of the refractive index profile from the assumed symmetry leads to a more complex transverse mode spectrum which is not possible to describe with the previous approach. In fact three different kinds of problems: electrical, thermal and optical have to be solved considering their mutual couplings. For more details, see [62–64].
Finally, varying the bias current the output field will change in its shape and its frequency (red-shift) with possibly a different number of modes emitted. This last phenomenon is due, beyond the variation of the refractive index of the structure, by spatial hole burning  which cause the excitation of lateral modes. Figure 1.18 shows those effects for a MTM VCSEL.
850 851 852 853 854 855 856
0 100 200 300 400 500
1 mA 2 mA 3 mA 4 mA 5 mA 6 mA 7 mA
Figure 1.18: Example of spectrum variation changing the biasing current for a MTM VCSEL realized in GaAs.
1.3.3 SiGe HPT technology